The so-called graphane is a fully hydrogenated form of graphene. Because it is fully hydrogenated, graphane is expected to have a wide bandgap and is theoretically an electrical insulator. The transition from graphene to graphane is that of an electrical conductor, to a semiconductor, and ultimately to an electrical insulator. This unique characteristic of graphane has recently gained both academic and industrial interest. Towards the end of developing novel applications of this important class of nanoscale material, computational modeling work has been carried out by a number of theoreticians to predict the structures and electronic properties of graphane. At the same time, experimental evidence has emerged to support the proposed structure of graphane. This review article covers the important aspects of graphane including its theoretically predicted structures, properties, fabrication methods, as well as its potential applications.
Graphene was first discovered in 2004 by Novoselov et al. . Graphene is a single atomic layer with a thickness of only 0.34 nm of sp2 hybridized carbon atoms covalently bonded to three other atoms arranged in a honeycomb lattice [1–7]. Graphene's unique structural, mechanical, and electrical properties and high carrier mobility makes it one of the most important topics in materials science today [8–14]. Graphene forms the basic structure of other carbon-based materials such as fullerene (wrapped-up graphene) [15–21], carbon nanotubes (several graphene sheets rolled up along a vertical axis) [22–29], and graphite (stacked graphene) [30–35]. Some of the carbon-based materials are illustrated in Figure 1.
Graphene has unique properties with tremendous potential applications, such as chemical sensors [36, 37], nanoelectronic devices , hydrogen storage systems , or polymer nanocomposites . Graphene could be considered as a prototypical material to study the properties of other two-dimensional nanosystems. Several two-dimensional structures have been explored in the literature [41, 42]. Graphene-like two-dimensional silicon carbide [43, 44], silicon [45, 46], germanium [47, 48], boron nitride [49, 50], and zinc oxide  have been explored in the literature.
One important development since the discovery of graphene is the discovery of the so-called graphane, which is a fully hydrogenated form of graphene, as shown in Figure 2. In this form, all carbon atoms in this fully hydrogenated form assume in the sp3 hybridization. This novel material, graphane, was first proposed by Lu et al. in theoretical investigation , and the predicted graphane structure was later confirmed by an experiment by Elias et al. . It was reported that graphene was changed into a new structure called graphane by exposing graphene to hydrogen plasma for several hours. Graphane is predicted to be a stable structure consisting of a graphene layer in which each C atom is sp3-bonded to one H atom above and below the C atom in an alternating manner . Graphane is predicted to have a bandgap of about 3.5 eV and has potential applications in electronics. In addition to forming graphane, hydrogen plasma exposure was observed to form partially hydrogenated graphene, which consisted of a graphene layer in which only one side was hydrogenated. Although hydrogenation of only one side of graphene is not predicted to be stable, it is proposed that ripples in graphene, which have sp3-like bonding angles, facilitate the sp3 bonding of C with H on only one side of the graphene. Partially hydrogenated graphene is observed to be insulating and thus has potential applications in electrical isolation for graphene-based circuits .
This review article is intended to focus on the fabrication and structure features of graphane (or graphane-like [54, 55]) and the potential application of graphane (or graphane-like) and properties. It covers the latest developments and new perspectives of graphane-based hydrogen storage  and transistor  with the special discussions on the merits and limitations of the material. Except for presenting a brief overview of the synthesis processes of single-layer graphane, graphane-like, graphene-graphane, graphane nanoribbons [58, 59], respectively, the structure features of graphane, particularly related to hydrogen storage and transistor, have been discussed.
Computational modeling of graphane
Flores et al.  used ab initio quantum calculations in order to optimize the geometry of graphane-like structures. They used classical reactive bond-order approach in order to investigate the effects of hydrogenation on geometrical structures for a number of graphene membrane models. Molecular dynamics (MD) simulations were used to address the dynamics of hydrogen incorporation into graphene membranes. As the results are displayed, H frustration were very likely to occur, perfect graphane-like structures are unlikely to be formed, and hydrogenated domains are very stable (relevant parameter and crystalline structures shown in Table 1 and Figure 3).
Dora et al.  used density functional theory, which studies the density of states in monolayer graphene (MLG) and bilayer graphene (BLG) at low energies in the presence of a random symmetry-breaking potential. And it had a breaking potential, which opens a uniform gap, and a random symmetry-breaking potential also created tails in the density of states.
Experimental synthesis of graphane
The transition from graphene to graphane is that of an electrical conductor to a semiconductor and ultimately to an insulator, which is dependent upon the degree of hydrogenation.
In 2009, the graphane was synthesized by exposing the single-layer graphene to a hydrogen plasma .
Savchenko  used hydrogen plasma to react with graphene for the preparation of graphane and the preparation process was shown in Figure 4. This method was not able to control the degree of hydrogenation.
Wang et al.  reported a new route to prepare high-quality and monolayer graphane by plasma-enhanced chemical vapor deposition (the structures model as shown in Figure 5). A large-area monolayer graphane-like film was produced by remote-discharged radio frequency plasma beam deposition at 650°C on Cu/Ti-coated SiO2-Si. The advantages of the plasma deposition were very short deposition time (<5 min) and very low growth temperature of 650°C compared to the current thermal chemical vapor deposition approach (1,000°C).
Structures of graphane
Many configurations with low energies for graphane were proposed. Sluiter et al.  and Sofo et al.  reported that the most stable configuration of graphane was the chair-like structure, with the UDUDUD hydrogenation in each hexagonal carbon ring as shown in Figure 6a . Sluiter et al. , Leenaerts et al. , and Bhattacharya et al.  reported that the second stable configuration was the 'stirrup’ with the UUUDDD hydrogenation in each carbon ring shown in Figure 6a, whose energy was about 28 meV/atom larger than that of the chair one. At the point of stability, the following configurations for graphane allotropes are boat-1 [63, 64, 66] with the UUDDUU hydrogenation, boat-2 [65, 66] with the UUUUDD hydrogenation, twist-boat  with the UUDUDD hydrogenation and other configurations with relatively high energies which were reported in the literatures [65, 69]. Recently, He et al.  used the restrictive condition of keeping the hexagonal hydrocarbon rings equivalent in the systems, and proposed a tricycle graphane allotrope in which each hexagonal hydrocarbon ring with the same UUUDUD hydrogenation was equivalent, as shown in Figure 6b. Table 2 summarizes the structure information for the six fundamental allotropes of graphane .
Xue and Xu  used a first-principle approach to study strain effects on basal-plane hydrogenation of graphene. Figure 7 shows the predicted energy of both types of graphane structures and also the combined system of pristine graphene and isolated hydrogen atom. The results also show that the in-plane modulus of graphene C = d2E / Adϵ2 = 1,260 GPa is reduced by 52% and 26% in symmetric and antisymmetric phases, respectively, where E is the potential energy, ϵ is the in-plane biaxial strain, and A is the calculated cross-sectional area where the thickness of graphene is taken as 3.4 Å. Accordingly, the biaxial tensile strength has a strong reduction after hydrogenation, from 101.27 GPa to 49.64 and 67.92 GPa due to the hydrogenation-induced rehybridization.
Popova and Sheka  used quantum-mechanochemical-reaction-coordinate simulations to investigate the mechanical properties of hydrogen functionalized graphene. Their results showed that the mechanical behavior of graphane was anisotropic so that tensile deformation occurred quite differently along (zg mode) and normally (ach mode) to the C-C bonds chain. The tensile strengths at fracture constituted 62% and 59% of graphene for the ach and zg modes, respectively, while the fracture strains increased by 1.7 and 1.6 times. Young's modules of the two deformation modes of graphane decreased by 1.8 and 2 times. Some mechanical parameters are shown in Table 3.
Peng et al.  investigated the effect of the hydrogenation of graphene to graphane on its mechanical properties using first-principles calculations based on the density functional theory. The results show that graphane exhibits a nonlinear elastic deformation up to an ultimate strain, which is 0.17, 0.25, and 0.23 for armchair, zigzag, and biaxial directions, respectively, and also have a relatively low in-plane stiffness of 242 N/m2, which is about 2/3 of that of graphene, and a very small Poisson ratio of 0.078, 44% of that of graphene. There has been a good idea which states that such unique mechanical properties make the graphane a good candidate for materials used in building the tubes or pipelines that transfer materials in high speed under applied high pressure.
Ao et al.  used the density functional theory to investigate the thermal stability of graphene/graphane nanoribbons (GGNRs). They found that the energy barriers for the diffusion of hydrogen atoms on the zigzag and armchair interfaces of GGNRs were 2.86 and 3.17 eV, respectively, while the diffusion barrier of an isolated H atom on pristine graphene was only approximately 0.3 eV. These results unambiguously demonstrated that the thermal stability of GGNRs could be enhanced significantly by increasing the hydrogen diffusion barriers through graphene/graphane interface engineering. Similarly, Costamagna et al.  used large scale atomistic simulations to study the thermal fluctuations of graphane. Rajabpour et al.  used nonequilibrium molecular dynamics simulations to investigate the thermal conductivity of hybrid graphene-graphane nanoribbons. Neek-Amal and Peeters  used atomistic simulations to determine the roughness and the thermal properties of a suspended graphane sheet. Compared with graphene, graphane had a larger thermal contraction, a wide range corresponding to length scales in the range 30 to 125 Ǻ at room temperature. The estimated heat capacity was 29.32 ± 0.23 J/mol.K which was 14.8% larger than the one for graphene.
In addition, graphane or graphane-like structures have magnetic properties and thermal performance. Neek-Amal and Peeters  investigated the lattice thermal properties of graphane, including thermal contraction, roughness, and heat capacity. Results showed that the roughness, amplitude, and wave lengths of the ripples were very different. The thermal contraction effect of graphane is larger than for graphene. Above 1,500 K, graphane is buckled and starts to lose H atoms at the edges of the membrane. Roughness of graphane is larger than that of graphene and the roughness exponent in graphene decreases versus temperature (from 1.2 to 1.0), while for graphane, it stays around 1.0 implying random uncorrelated roughness. Heat capacity of graphane is found to be 14.8%, which is larger than that of graphene.
In Universal optical properties of graphane nanoribbons: A first-principles study by Yang et al. , the results indicated that the optical properties of graphane nanoribbons were independent of their edge shapes and widths. Their unique optical properties make graphane nanoribbons suitable for various applications in nanoscale optical and optoelectronic devices.
León and Pacheco  studied on the electronic and dynamical properties of a molecular wire consisting of molecules with structures of graphane and a graphane nanoribbon. Bubin and Varga  had discussed the response of graphene and graphane fragments to strong femtosecond laser pulses and the results showed that the hydrogenation was controllable by strong femtosecond laser pulses. Before that, Chandrachud et al.  had been systematic studied on electronic structure from graphene to graphane. Simultaneously, their results revealed that it was possible to design a pattern of hydrogenation so as to yield a semiconducting sheet with a bandgap much lower than that of graphane. Nanyang Technological University's Hwee Ling Poh et al.  investigated the electrochemical behavior of hydrogenated graphene synthesized under various pressures and temperatures for comparison and showed that hydrogenation of graphene (towards graphane) resulting in a decrease in the observed heterogeneous electron transfer rates as measured by cyclic voltammetry and an increase in the charge transfer resistance as measured by impedance spectroscopy as compared to graphene.
Lee and Grossman  used the first-principles calculations based on the density functional theory (DFT) to explore the magnetic properties of graphene-graphane superlattices with zigzag interfaces and separately varying widths. The results displayed that the magnetic properties of the superlattices were entirely determined by the graphene region due to the π character of the spin density. It was a potential for future spintronics applications with a variable spin-current density. Berashevich and Chakraborty , Schmidt and Loss , Şahin et al. , and Hernández et al.  also did the related research on the magnetism of graphane, such as sustained ferromagnetism, tunable edge magnetism, magnetization of graphane by dehydrogenation, graphane nanoribbons magnetic, and so on.
Derivatives of graphane
Graphene can be functionalized by varied methods. Haldar et al.  used Fe to replace the hydrogen on the plane of graphane. The work showed that the response of the two channels, the armchair and the zigzag channels, were different. Hussain  and AlZahrani  reported the strain induced lithium functionalized graphane as a high-capacity hydrogen storage material and used the manganese adsorption graphene and graphane as magnetic materials. Graphane's derivatives were not only just about functionalization of the surface atoms, but also by changing the substrate atoms to achieve its function. For example, Lu et al. , from the University of Science and Technology of China, studied the chemical modification with –OH or -NH2 group on planar polysilane and graphane. Hőltzl et al. , Artyukhov and Chernozatonskii , Bianco , Garcia et al.  reported separately in cis-polyacetylene and graphane, carbon monofluoride and graphane, germanium graphane analogue, group-IV graphene, graphane-like nanosheets, and so on.
Therefore, we can fabricate many derivatives of graphane by changing the substrate atoms (like C, Si, Ge, P) and the surface atoms (like H, –OH, -NH2, He, Li, Fe, Mn, and all the VII A element).
Applications of graphane
As mentioned in many articles, graphane or graphane-like materials can be applied in many fields. Nechae  considered the thermodynamic and experimental backgrounds of the condensed hydrogen storage problem, and an effective method was put forward to produce a high-density hydrogen carrier which was hydrogen intercalation in carbonaceous nanomaterials at relevant temperatures and pressures (at the cost of the hydrogen association energy). The result displayed the intercalated solid molecular hydrogen in graphane-like nanofibers (17 wt.% H2). Compared with the US Department of Energy (DOE)'s strategic objectives for the year 2015 which include a minimum 'gravimetric’ capacity (weight of stored H2/system weight) of 9.0 wt.% of reversible hydrogen and a 'volumetric’ capacity (density) of 0.081 g(H2)/cm3(system), graphane-like nanofibers are much more acceptable and efficient hydrogen storage technology.
Gharekhanlou et al.  reported that graphane materials can be used as bipolar transistor. Cudazzo et al.  provided an exact analytic form of the two-dimensional screened potential. Gharekhanlou et al.  introduced a 2D p-n junction based on graphane with hydrogen deficiency to reduce the bandgap effectively. And using basic analysis has shown that within the approximation of Shockley law of junctions, an exponential ideal I-V characteristic is expectable. This broadens the graphane or graphane-like application in transistor devices. Savini et al.  used p-doped graphane to fabricate a prototype high-Tc electron–phonon superconductor, which has Tc as high as 150 K for a 1-nm nanowire, higher than copper oxides. Loktev and Turkowski  and Kristoffel and Rägo  considered the superconducting properties of multilayer graphane by taking into account the fluctuations of the order parameter. The result showed that in the single-layer case, the BKT critical temperature which corresponds to the vortex SC is equal to the MF temperature 100 K beginning from a rather low value of doping less than 0.01. And they estimated that the critical temperature may reach values 150 K, which is significantly higher than the maximal temperature under ambient pressure in cuprates. Nechaev  said that the high-density hydrogen carrier intercalation in graphane-like nanostructures can be used in fuel cell-powered vehicles. Hussian et al. [104, 105] used polylithiated (OLi2) functionalized graphane as a potential hydrogen storage material, the storage capacity to achieve 12.9 wt.%.
Exceptional physical properties, chemical tunability, potential electronic, and transistor applications of graphane have definitely gained the interest of materials and electronics researchers. This review article is intended to focus on the fabrication and structural features of graphane (or graphane-like material) and the potential applications of graphane (or graphane-like) and graphane-based nanocomposites. It covers the latest advancement and new perspectives of graphane as a potential material for hydrogen storage and transistor with the special discussions on the merits and limitations of the material. After presenting a brief overview of the synthesis processes of single-layer graphane, graphane-like, graphene-graphane, and graphane nanoribbons, the structure features of graphane, particularly related to the hydrogen storage and transistor, have been discussed.
By reversible hydrogenation, one can make the graphene material from conductor to insulator. Thus, we can control the degree of hydrogenation to modulate the conductive properties. Through this process, graphene-graphane mixed structures offer greater possibilities for the manipulation of the material's semiconducting properties and they can be potentially applied in the field of transistor, electron–phonon superconductor and others applications. The behavior of graphene to graphane or graphane to graphene is the progress of hydrogen energy storage or release. Graphane or graphane-like material can be used as hydrogen storage material for fuel cells. Because of its wide range of conductivity, it can be used for nanosensors with exceptional sensitivity.
Certainly, most notably we can fabricate many derivatives of graphane by changing the substrate atoms (like C, Si, Ge, P, S) and the surface atoms (like H, –OH, -NH2, He, Li, Fe, Mn, Ag, and all the VII A element) so as to promote its application value and expand the application field.
Novoselov KS, Geim AK, Morozov SV, Jiang D, Zhang Y, Dubonos SV, Grigorieva IV, Firsov AA: Electric field effect in atomically thin carbon films. Sci 2004, 306: 666. 10.1126/science.1102896
Layek RK, Nandi AK: A review on synthesis and properties of polymer functionalized graphene. Polymer 2013, 54: 5087. 10.1016/j.polymer.2013.06.027
Geim AK, Novoselov KS: The rise of graphene. Nat Mater 2007, 6: 183. 10.1038/nmat1849
Hill EW, Vijayaragahvan A, Novoselov K: Graphene sensors. IEEE Sensors J 2011, 113: 161.
Si Y, Samulski ET: Synthesis of water soluble graphene. Nano Lett 2008, 8: 1679. 10.1021/nl080604h
Choi W, Lahiri I, Seelaboyina R, Kang YS: Synthesis of graphene and its applications: a review. Crit Rev Solid State Mater Sci 2010, 35: 52. 10.1080/10408430903505036
Singh V, Joung D, Zhai L, Das S, Khondaker SI, Seal S: Graphene based materials: past, present and future. Prog Mater Sci 2011, 56: 1178. 10.1016/j.pmatsci.2011.03.003
Castro Neto AH, Guinea F, Peres NM, Novoselov KS, Geim AK, Rev , Mod : The electronic properties of graphene. Phys 2009, 81: 109.
Basua S, Bhattacharyya P: Recent developments on graphene and graphene oxide based solid state gas sensors. Sens Actuators B 2012, 173: 1.
Gomez De Arco L, Zhang Y, Schlenker CW, Ryu K, Thompson ME, Zhou C: Continuous, highly flexible, and transparent graphene films by chemical vapor deposition for organic photovoltaics. ACS Nano 2010, 4: 2865. 10.1021/nn901587x
Zhu Y, Murali S, Cai W, Li X, Suk JW, Potts JR, Ruoff RS: Graphene and graphene oxide: synthesis, properties and applications. Adv Mater 2010, 22: 3906. 10.1002/adma.201001068
Allen MJ, Tung VC, Gomez De Arco L, Xu Z, Chen LM, Nelson KS, Zhou C, Kaner RB, Yang Y: Soft transfer printing of chemically converted graphene. Adv Mater 2009, 21: 2098. 10.1002/adma.200803000
Gorbachev RV, Mayorov AS, Savchenko AK, Horsell DW, Guinea F: Conductance of p-n-p graphene structures with air-bridge top gates. Nano Lett 1995, 2008: 8.
Dragoman M, Dragoman D: Graphene-based quantum electronics. Prog Quantum Electron 2009, 33: 165. 10.1016/j.pquantelec.2009.08.001
Craciun MF, Russo S, Yamamoto M, Tarucha S: Tuneable electronic properties in graphene. Nano Today 2011, 6: 42. 10.1016/j.nantod.2010.12.001
Wintterlin J, Bocquet ML: Graphene on metal surfaces. Surf Sci 1841, 2009: 603.
Novoselov KS, Geim AK, Morozov SV, Jiang D, Katsnelson MI, Grigorieva IV, Dubonos SV, Firsov AA: Two-dimensional gas of mass less Dirac fermions in graphene. Nature 2005, 438: 197. 10.1038/nature04233
Zhang Y, Tan YW, Stormer HL, Kim P: Experimental observation of the quantum Hall effect and Berry’s phase in graphene. Nature 2005, 438: 201. 10.1038/nature04235
Inagaki M, Kim YA, Endo M: Graphene: preparation and structural perfection. J Mater Chem 2011, 21: 3280. 10.1039/c0jm02991b
Nair RR, Blake P, Grigorenko AN, Novoselov KS, Booth TJ, Stauber T, Peres NMR, Geim AK: Fine structure constant defines visual transparency of graphene. Science 2008, 320: 1308. 10.1126/science.1156965
Acik M, Chabal YJ: Nature of graphene edges: a review. Jpn J Appl Phys 2011, 50: 070101.
Kim KS, Zhao Y, Jang H, Lee SY, Kim JM, Kim KS, Ahn JH, Kim P, Choi J, Hong BH: Large-scale pattern growth of graphene films for stretchable transparent electrodes. Nature 2009, 457: 706. 10.1038/nature07719
Lee C, Wei X, Kysar JW, Hone J: Measurement of the elastic properties and intrinsic strength of monolayer graphene. Science 2008, 321: 385. 10.1126/science.1157996
Cheianov VV, Falko V, Altshuler BL: The focusing of electron flow and a Veselago lens in graphene p-n junctions. Science 2007, 315: 1252. 10.1126/science.1138020
Geim AK: Graphene: status and prospects. Science 2009, 324: 1530. 10.1126/science.1158877
Booth TJ, Blake P, Nair RR, Jiang D, Hill EW, Bangert U, Bleloch A, Gass M, Novoselov KS, Katsnelson MI, Geim AK: Macroscopic graphene membranes and their extraordinary stiffness. Nano Lett 2008, 8: 2442. 10.1021/nl801412y
Pati SK, Enoki T, Rao CNR: (Eds): Graphene and Its Fascinating Attributes. Singapore: World Scientific Publishing Co Pte. Ltd; 2011.
Tombros N, Jozsa C, Popinciuc M, Jonkman H, van Wees B: Electronic spin transport and spin precession in single graphene layers at room temperature. Nature 2007, 448: 571. 10.1038/nature06037
Raza H: (Ed): Graphene Nanoelectronics: Metrology, Synthesis Properties and Applications. Berlin, Germany: Springer; 2012.
Kuila T, Bose S, Khanra P, Mishra AK, Kim NH, Lee JH: Recent advances in graphene-based biosensors. Biosens Bioelectron 2011, 26: 4637. 10.1016/j.bios.2011.05.039
Choi W, Lee JW: Graphene: Synthesis and Applications. New York, USA: CRC Press (Taylor and Francis group); 2012.
Chan HE: (Ed): Graphene and Graphite Materials. New York, USA: Nova Science Publishers Inc; 2010.
Pumera M, Ambrosi A, Bonanni A, Chng ELK, Poh HL: Graphene for electrochemical sensing and biosensing. Trends Anal Chem 2010, 29: 954. 10.1016/j.trac.2010.05.011
Lang B: A LEED study of the deposition of carbon on platinum crystal surfaces. Surf Sci 1975, 53: 317. 10.1016/0039-6028(75)90132-6
Basu S, Bhattacharyya P: Recent developments on graphene and graphene oxide based solid state gas sensors. Sens Actuators B 2012, 173: 21.
Pumera M: Electrochemistry of graphene: new horizons for sensing and energy storage. Chem Rec 2009, 9: 211. 10.1002/tcr.200900008
Casolo S, Martinazzo R, Tantardini GFJ: Band engineering in graphene with superlattices of substitutional defects. Phys Chem C 2011, 115: 3250. 10.1021/jp109741s
Schwierz F: Graphene transistors. Nature Nanotech 2010, 5: 487. 10.1038/nnano.2010.89
Boukhvalov DW, Katsnelson MI, Lichtenstein AI: Hydrogen on graphene: electronicstructure, total energy, structural distortions and magnetism from first-principles calculations. Phys Rev B 2008, 77: 405.
Kuilla T, Bhadra S, Yao D, Kim NH, Bose S, Lee JH: Recent advances in graphene based polymer composites. Prog Polym Sci 2010, 35: 1350. 10.1016/j.progpolymsci.2010.07.005
Lu N, Li Z, Yang J: Electronic structure engineering via on-plane chemical functionalization: a comparisonstudy on two-dimensional polysilane and graphane. Phys Chem C 2009, 113: 16741. 10.1021/jp904208g
Elias DC, Nair RR, Mohiuddin TMG, Morozov SV, Blake P, Halsall MP, Ferrari AC, Boukhvalov DW, Katsnelson MI, Geim AK, Novoselov KS: Control of graphene's properties by reversible hydrogenation: evidence for graphane. Science 2009, 323: 610. 10.1126/science.1167130
Huda MN, Yan YF, Al-Jassim M, Chem M: Thermal conductivity of silicon and carbon hybrid monolayers: a molecular dynamics study. Phys Lett 2009, 479: 25.
Bekaroglu E, Topsakal M, Cahangirov S, Ciraci S: First-principles study of defects and adatoms in silicon carbide honeycomb structures. Phys Rev B 2010, 81: 075433.
Nakano H, Mitsuoka T, Harada M, Horibuchi K, Nozaki H, Takahashi N, Nonaka T, Seno Y, Angew NH: Epitaxial growth of a silicene sheet. Chem 2006, 118: 6451.
Voon LCLY, Sandberg E, Aga RS, Farajian AAA: Hydrogen compounds of group-IV nanosheets. Phys Lett 2010, 97: 163114.
Cahangirov S, Topsakal M, Akturk E, Sahin H, Ciraci S: Two-and one-dimensional honeycomb structures of silicon and germanium. Phys Rev Lett 2009, 102: 236804.
Houssa M, Pourtois G, Afanasév VV, Stesmans AA: Electronic properties of two-dimensional hexagonal germanium. Phys Lett 2010, 96: 082111.
Tang SB, Cao ZX: Structural and electronic properties of the fully hydrogenated boron nitride sheets and nanoribbons: insight from first-principles calculations. Chem Phys Lett 2010, 488: 67. 10.1016/j.cplett.2010.01.073
Topsakal M, Aktürk E, Ciraci S: First-principles study of two-and one-dimensional honeycomb structures of boron nitride. Phys Rev B 2009, 79: 115442.
Zhang Y, Wu SQ, Wen YH, Zhu ZZA: Surface-passivation-induced metallic and magnetic properties of ZnO graphitic sheet. Phys Lett 2010, 96: 223113.
Wen X-D, Yang T, Hoffmann R, Ashcroft NW, Martin RL, Rudin SP, Zhu J-X: Graphane nanotubes. ACS Nano 2012, 8: 7142.
Jones JD, Mahajan KK, Williams WH, Ecton PA, Mo Y, Perez JM: Formation of graphane and partially hydrogenated graphene by electron irradiation of adsorbates on graphene. Carbon 2010, 48: 2335. 10.1016/j.carbon.2010.03.010
Lueking D, Gutierrez HR, Fonseca DA, Narayanan DL, Essendelft DV, Jain P, Cliord CEB: Graphene to graphane: a theoretical study. J Amer Chem Soc 2006, 128: 7758. 10.1021/ja0604818
Ray NR, Srivastava AK, Grotzschel R: In search of graphane - a two-dimensional hydrocarbon. Cond Mat Mtrl Sci 2008, arXiv: 0802–3998v1.
Elias DC, Nair RR, Mohiuddin TMG, Morozov SV, Blake P, Halsall MP, Ferrari AC, Boukhvalov DW, Katsnelson MI, Geim AK, Novoselov KS: Control of graphene's properties by reversible hydrogenation: evidence for graphane. Sci 2009, 30323: 610.
Savchenko A: Transforming graphene. Sci 2009, 323: 589. 10.1126/science.1169246
Tozzini V, Pellegrini V: Electronic structure and Peierls instability in graphene nanoribbons sculpted in graphane. Phys Rev B 2010, 81: 113404.
Ao ZM, Hernández-Nieves AD, Peeters FM, Li S: Enhanced stability of hydrogen atoms at the graphene/graphane interface of nanoribbons. Appl Phys Lett 2010, 97: 256.
Flores MZS, Autreto PAS, Legoas SB, Galvao DS: Graphene to graphane: a theoretical study. Nanotechnol 2009, 20: 465704. 10.1088/0957-4484/20/46/465704
Dora B, Ziegler K: Gaps and tails in graphene and graphane. New J Phys 2009, 11: 095006. 10.1088/1367-2630/11/9/095006
Wang Y, Xu X, Lu J, Lin M, Bao Q, Ozyilmaz B, Loh KP: Toward high throughput interconvertible graphane-to-graphene growth and patterning. Nano 2010, 4: 6146.
Sluiter MHF, Kawazoe : Cluster expansion method for adsorption: Application to hydrogen chemisorption on graphene. Phys Rev B 2003, 68: 085410.
Sofo JO, Chaudhari AS, Barber GD: Graphane: a two-dimensional hydrocarbon. Phys Rev B 2007, 75: 153401.
Wen XD, Hand L, Labet V, Yang T, Hoomann R, Ashcroft NW, Oganov AR, Lyakhov O: Benzene under high pressure: a story of molecular crystals transforming to saturated networks, with a possible intermediate metallic phase. Proc Natl Acad Sci 2011, 108: 6833. 10.1073/pnas.1103145108
Leenaerts O, Peelaers H, Hernández-Nieves AD, Partoens B, Peeters FM: First-principles investigation of graphene fluoride and graphane. Phys Rev B 2010, 82: 195436.
Bhattacharya A, Bhattacharya S, Majumder C, Das GP: Third conformer of graphane: a first-principles density functional theory study. Phys Rev B 2011, 83: 033404.
Samarakoon DK, Chen ZF, Nicolas C, Wang XQ: Structural and electronic properties of fluorographene. Small 2011, 7: 965. 10.1002/smll.201002058
Samarakoon DK, Wang XQ: Chair and twist-boat membranes in hydrogenated graphene. ACS Nano 2009, 12: 4017.
He C, Sun LZ, Zhang CX, Jiao N, Zhang KW, Zong J: Structure, stability and electronic properties of tricycle type graphane. Phys Status Solidi (RRL) -Rapid Research Letters 2012, 6: 427. 10.1002/pssr.201206358
Xue K, Xu Z: Strain effects on basal-plane hydrogenation of graphene: a first-principles study. Appled Phys Lett 2010, 96: 063103. 10.1063/1.3298552
Popova NA, Sheka EF: Mechanochemical reaction in graphane under uniaxial tension. Researchgate 2011, 06arXiv: 01.
Peng Q, Liang C, Ji W, De S: A theoretical analysis of the effect of the hydrogenation of graphene to graphane on its mechanical properties. Phys Chem Chem Phys 2003, 2013: 15.
Ao ZM, Hernández-Nieves AD, Peeters FM, Li S: Enhanced stability of hydrogen atoms at the graphene/graphane interface of nanoribbons. Appl Phys Lett 2010, 97: 233109. 10.1063/1.3525377
Costamagna S, Neek-Amal M, Los JH, Peeters FM: Thermal rippling behavior of graphane. Phys Rev B(R) 2012, 86: 041408.
Rajabpour A, Vaez Allaei SM, Kowsary F: Interface thermal resistance and thermal rectification in hybrid graphene-graphane nanoribbons: a nonequilibrium molecular dynamics study. Appled Phys Lett 2011, 99: 051917. 10.1063/1.3622480
Neek-Amal M, Peeters FM: Lattice thermal properties of graphane: thermal contraction, roughness and heat capacity. Phys Rev B 2011, 83: 235437.
Neek-Amal M, Peeters FM: Lattice thermal properties of graphane: thermal contraction, roughness and heat capacity. Rev B 2011, 83: 16.
Yang Y-E, Yang Y-R, Yan X-H: Universal optical properties of graphane nanoribbons: a first-principles study. Phys E 2012, 44: 1406. 10.1016/j.physe.2012.03.002
León A, Pacheco M: Electronic and dynamics properties of a molecular wire of graphane Nanoclusters. Phys Lett A 2011, 375: 4190. 10.1016/j.physleta.2011.09.044
Bubin S, Varga K: Electron and ion dynamics in graphene and graphane fragments subjected to high-intensity laser pulses. Physical review B 2012, 85: 205441.
Chandrachud P, Pujari BS, Haldar S, Sanyal B, Kanhere DG: A systematic study of electronic structure from graphene to graphane. Phys Condens Matter 2010, 22: 465502. 10.1088/0953-8984/22/46/465502
Poh HL, Sofer Z, Pumera M: Graphane electrochemistry: electron transfer at hydrogenated graphenes. Electrochem Commun 2012, 25: 58.
Lee J-H, Grossman JC: Magnetic properties in graphene-graphane superlattices. Applied Physic Lett 2010, 97: 97.
Berashevich J, Chakraborty T: Sustained ferromagnetism induced by H-vacancies in graphane. Nanotechnology 2010, 21: 355201. 10.1088/0957-4484/21/35/355201
Schmidt MJ, Loss D: Tunable edge magnetism at graphene/graphane interfaces. Phys Rev B 2010, 82: 085422.
Şahin H, Ataca C, Ciraci S: Magnetization of graphane by dehydrogenation. Appl Phys Lett 2009, 95: 222510. 10.1063/1.3268792
Hernández-Nieves AD, Partoens B, Peeters FM: Electronic and magnetic properties of superlattices of graphene/graphane nanoribbons with different edge hydrogenation. Phys Rev B 2010, 82: 165412.
Haldar S, Kanhere DG, Sanyal B: Magnetic impurities in graphane with dehydrogenated channels. Phys Rev B 2012, 85: 155426.
Hussain T, DeSarkar A, Ahuja R: Strain induced lithium unctionalized graphane as a high capacity hydrogen storage material. Phys Lett 2012, arXiv: 5228.
AlZahrani AZ: Theoretical investigation of manganese adsorption on graphene and graphane: A first-principles comparative study. Physica B 2012, 407: 992. 10.1016/j.physb.2011.12.127
Hőltzl T, Veszprémi T, Nguyen MT: Phosphaethyne polymers are analogues of cis-polyacetylene and graphane. C. R. Chimie 2010, 13: 1173. 10.1016/j.crci.2010.03.033
Artyukhov VI, Chernozatonskii LA: Structure and Layer interaction in carbon monofluoride and graphane: a comparative computational study. Phys Chem A 2010, 114: 5389. 10.1021/jp1003566
Bianco E: Stability and exfoliation of germanane: a germanium graphane analogue. ACS Nano 2013, 7: 4414. 10.1021/nn4009406
Garcia JC, De Lima DB, Assali LVC, Justo JF: Group-IV graphene and graphane-like nanosheets. Phys Chem C 2011, 115: 13242. 10.1021/jp203657w
Nechae YS: On the solid hydrogen carrier intercalation in graphane-like regions in carbon-based nanostructures. Int J Hydrog Energy 2011, 36: 9023. 10.1016/j.ijhydene.2011.04.073
Gharekhanlou B, Tousaki SB, Khorasani S: Bipolar transistor based on graphane. Phys. Conf. Ser 2010, 248: 012061.
Cudazzo P, Tokatly IV, Rubio A: Dielectric screening in two-dimensional insulators: implications for excitonic and impurity states in graphane. Phys Rev B 2011, 84: 085406.
Gharekhanlou B, Khorasani S, Senior Member: Current–voltage characteristics of graphane p-n junctions. Electron Devices 2010, 57: 209.
Savini A, Ferrari C, Giustino F: Doped graphane: a prototype high-Tc electron–phonon superconductor. Phys Rev Lett 2010, 105: 037002.
Loktev VM, Turkowski V: Possible high-temperature superconductivity in multilayer graphane: can the cuprates be beaten? Low Temp Phys 2011, 164: 264.
Kristoffel N, Rägo K: On the interband pairing in doped graphane. Phys Lett A 2011, 375: 2246. 10.1016/j.physleta.2011.04.038
Nechaev YS: The high-density hydrogen carrier intercalation in graphane-like nanostructures, relevance to its on-board storage in fuel-cell-powered vehicles. The Open Fuel Cells J 2011, 4: 16. 10.2174/1875932701104010016
Hussain T, Maark TA, De Sarkar A, Ahuja R: Polylithiated (OLi2) functionalized graphane as a potential hydrogen storage material. Phys Chem 2012, 13: 1207–5385.
Hussain T, De Sarkar A, Ahuja R: Strain induced lithium functionalized graphane as a high capacity hydrogen storage material. Appl Phys Lett 2012, 101: 103907. 10.1063/1.4751249
This work was supported by the Shanghai Major Construction Projects (11XK18B, XKCZ1205), Shanghai Science and Technology Capacity Building Project Local Universities (11490501500), and Shanghai University of Engineering Science Innovation Project (13KY0410).
The authors declare that they have no competing interests.
SC and JL designed the structure and modified the manuscript articles; CZ drafted the manuscript. JW, QY, CL, DH, and TZ participated in the sequence alignment. All authors read and approved the final manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 2.0 International License ( https://creativecommons.org/licenses/by/2.0 ), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
About this article
Cite this article
Zhou, C., Chen, S., Lou, J. et al. Graphene’s cousin: the present and future of graphane. Nanoscale Res Lett 9, 26 (2014). https://doi.org/10.1186/1556-276X-9-26
- Partially hydrogenated graphene